2 Civil Engineering Material Lecture # 2Civil Engineering MaterialCementDr. Attaullah ShahDepartment of Civil EngineeringSwedish College of Engineering and Technology-Wah Cantt.
3 INTRODUCTIONDefinition: “Cement is a crystalline compound of calcium silicates and other calcium compounds having hydraulic properties” (Macfadyen, 2006).
4 HistoryLime and clay have been used as cementing material on constructions through many centuries.Romans are commonly given the credit for the development of hydraulic cement, the most significant incorporation of the Roman’s was the use of pozzolan-lime cement by mixing volcanic ash from the Mt. Vesuvius with lime.Best know surviving example is the Pantheon in RomeIn 1824 Joseph Aspdin from England invented the Portland cement
5 History of cement and concrete The early days:Setting stone blocks without cementing themMud mixed with straw is the oldest cementing material used to bind dried bricks togetherPyramid of Cheops.
6 Cheops, GizaStones were brought from Aswan and Tura using the Nile riverBuilt around 2566 B.C.It would have taken over 2,300,000 blocks of stone with an average weight of 2.5 tons eachTotal weight of 6 million tons30 years and 100,000 slaves to build itHas a height of 482 feet (140m)It is the largest and the oldest of the Pyramids of GizaMortars made by calcining impure gypsum
7 History of cement and concrete Non-hydraulic cementsGypsum and limeCements based on compounds of lime (calcareous cements)GypsumCalcining impure gypsum at 130 °CAdd water calcined gypsum and water recombineCannot harden under water because gypsum is quite soluble.Pyramid of Cheops (3000 B.C.)
14 Types of CementCements are considered hydraulic because of their ability to set and harden under or with excess water through the hydration of the cement’s chemical compounds or minerals.There are two types:Those that activate with the addition of waterAnd pozzolanic that develop hydraulic properties when the interactwith hydrated lime Ca(OH)2Pozzolanic: any siliceous material that develops hydraulic cementitious properties when interacted with hydrated lime.HYDRAULIC CEMENTS:Hydraulic lime: Only used in specialized mortars. Made from calcination of clay-rich limestones.Natural cements: Misleadingly called Roman. It is made from argillaceous limestones or interbedded limestone and clay or shale, with few raw materials. Because they were found to be inferior to Portland, most plants switched.
15 Portland cement: Artificial cement Portland cement: Artificial cement. Made by the mixing clinker with gypsum in a 95:5 ratio.Portland-limestone cements: Large amounts (6% to 35%) of ground limestone have been added as a filler to a Portland cement base.Blended cements: Mix of Portland cement with one or more SCM (supplementary cemetitious materials) like pozzolanic additives.Pozzolan-lime cements: Original Roman cements. Only a small quantity is manufactured in the U.S. Mix of pozzolans with lime.Masonry cements: Portland cement where other materials have been added primarily to impart plasticity.Aluminous cements: Limestone and bauxite are the main raw materials. Used for refractory applications (such as cementing furnace bricks) and certain applications where rapid hardening is required. It is more expensive than Portland. There is only one producing facility in the U.S.
16 GEOLOGY (RAW MATERIALS) The fundamental chemical compounds to produce cement clinker are:Lime (CaO)Silica (SiO2)Alumina (Al2O3)Iron Oxide (Fe2O3)Raw materials used in the production of clinker cementFly ash: by-product of burning finely grounded coal either for industrial application or in the production of electricity
17 Clinker compounds in Type I portland cement (Macfadyen, 2006)
18 SOURCES OF CaCO3 Sedimentary deposits of marine origin (limestone) Marble (metamorphosed limestone)ChalkMarlCoralAragoniteOyster and clam shellsTravertineTuffLIMESTONESOriginate from the biological deposition of shells and skeletons of plants and animals.Massive beds accumulated over millions of years.In the cement industry limestone includes calcium carbonate and magnesium carbonate.Most industrial quality limestones is of biological origin.The ideal cement rock 77 to 78% CaCO3, 14% SiO2, 2.5% Al2O3, and 1.75% FeO3. Limestone with lower content of CaCO3 and higher content of alkalis and magnesia requires blending with high grade limestone(Macfadyen, 2006)(Kussmaul, 2003)
19 SOURCES OF ARGILLACEOUS MINERALS Argillaceous mineral resources:Clay and shale for alumina and silicaIron ore for ironOther natural sources of silica are and alumina are:Loess, silt, sandstone, volcanic ash, diaspore, diatomite, bauxiteShales, mudstones, and sandstones are typically interbedded with the limestone and were deposited as the inland waters and oceans covered the land masses. Clays are typically younger surface deposits(Macfadyen, 2006)
20 USES Uses Main use is in the fabrication of concrete and mortars Modern usesBuilding (floors, beams, columns, roofing, piles, bricks, mortar, panels, plaster)Transport (roads, pathways, crossings, bridges, viaducts, tunnels, parking, etc.)Water (pipes, drains, canals, dams, tanks, pools, etc.)Civil (piers, docks, retaining walls, silos, warehousing, poles, pylons, fencing)Agriculture (buildings, processing, housing, irrigation)
21 It competes in the construction industry with concrete substitutes: AluminaAsphaltClay brickFiberglassGlassSteelStone WoodSome materials like fly ash and ground granulated furnace slugs have good hydraulic properties and are being used as partial substitutes for Portland cement in some concrete applications
22 Data in thousand metric tons PRODUCTIONData in thousand metric tons
24 World production of hydraulic cement by region (http://pubs.usgs.gov/of/2005/1152/ pdf).
25 U.S production and consumption of portland cement (http://pubs.usgs.gov/of/2005/1152/ pdf)
26 PORTLAND CEMENT Chemical composition of Portland Cement: a) Tricalcium Silicate (50%)b) Dicalcium Silicate (25%)c) Tricalcium Aluminate (10%)d) Tetracalcium Aluminoferrite (10%)e) Gypsum (5%)
27 FUNCTION :TRICALCIUM SILICATE Hardens rapidly and largely responsible forinitial set & early strengthThe increase in percentage of this compoundwill cause the early strength of PortlandCement to be higher.A bigger percentage of this compound willproduces higher heat of hydration andaccounts for faster gain in strength.
28 FUNCTION :DICALCIUM SILICATE Hardens slowlyIt effects on strength increases occurs at agesbeyond one week .Responsible for long term strength
29 FUNCTION :TRICALCIUM ALUMINATE Contributes to strength development in thefirst few days because it is the first compoundto hydrate .It turns out higher heat of hydration and contributes to faster gain in strength.But it results in poor sulfate resitance and increases the volumetric shrinkage upon drying.
30 Cements with low Tricalcium Aluminate contents usually generate less heat, develophigher strengths and show greaterresistance to sulfate attacks.It has high heat generation and reactivewith soils and water containing moderateto high sulfate concentrations so it’s leastdesirable.
31 FUNCTION : TETRACALCIUM ALUMINOFERRITE Assist in the manufacture of Portland Cementby allowing lower clinkering temperature.Also act as a fillerContributes very little strength of concreteeventhough it hydrates very rapidly.Also responsible for grey colour of OrdinaryPortland Cement
32 Manufacture of Portland cement Raw materialsPreparation of materialsBurningFinal processingQuality control
33 Raw materialsLimestone (calcium carbonate) is a common source of calcium oxide.Iron-bearing aluminosilicates are the most common source of silica.Aluminum and iron oxides act as fluxing agents i.e. lower fusion temperature of part of the raw mix to a practical firing temperature
34 Preparation of Materials Crush the materials and store themBlend the materials and grind themStore them and do final blendingBlending – assure constant composition and predictable properties.Wet, dry, and semi-dry processesBurn the materialsGrind, blend, and store the materials
35 WET PROCESS Raw materials are homogenized by crushing, grinding and blending so that approximately80% of the raw material pass a No.200 sieve.The mix will be turned into form of slurry byadding % of water.It is then heated to about 2750ºF (1510ºC) inhorizontal revolving kilns (76-153m lengthand m in diameter.
36 Wet process is obsolete Natural gas, petroluem or coal are used forburning. High fuel requirement may make ituneconomical compared to dry process.Wet process is obsolete
37 DRY PROCESS Raw materials are homogenized by crushing, grinding and blending so that approximately80% of the raw material pass a No.200 sieve.Mixture is fed into kiln & burned in a dry stateThis process provides considerable savings infuel consumption and water usage but theprocess is dustier compared to wet processthat is more efficient than grinding.
38 DRY PROCES & WET PROCESS In the kiln, water from the raw material isdriven off and limestone is decomposed intolime and Carbon Dioxide.limestone lime + Carbon DioxideIn the burning zone, portion of the kiln, silicaand alumina from the clay undergo a solidstate chemical reaction with lime to producecalcium aluminate.silica & alumina + lime calcium aluminate
39 Burning process Sintering (become a coherent mass with no melting) Fusion (complete melting)Clinkering – only about ¼ of the charge is in the liquid stateKilnLong steel pipeLined with refractory brickInclined a few degreesRotated at 60 to 200 rev/hTypically 6 m (20 ft) in diameter and 180 m (600 ft) longTime in the kiln from 2 h (wet process) to 1 h (dry process) or even (20 min) modern heat exchangersFour processes take place in the kilnEvaporation 240 to 450 °C
40 Limestone decomposes (700 °C) – CO2 driven off Calcination 600 to 1100 °CClay decomposes (600 °C)Limestone decomposes (700 °C) – CO2 driven offFormation of initial compounds (1000 °C)Initial formation of C2S (1200 °C), formation of calcium aluminates and FerritesFormation of melt (flux compounds melt) (1350 °C)Clinkering – charge temperature is 1400 to 1600 °CFormation of C3SCoolingRate of cooling significantly affects the reactivity of the final cementKlinker
41 The rotation and shape of kiln allow the blend to flow down the kiln, submitting it togradually increasing temperature.As the material moves through hotter regionsin the kiln, calcium silicates are formedThese products, that are black or greenishblack in color are in the form of smallpellets, called cement clinkersCement clinkers are hard, irregular and ballshaped particles about 18mm in diameter.
43 The cement clinkers are cooled to about 150ºF (51ºC) and stored in clinker silos. When needed, clinker are mixed with 2-5%gypsum to retard the setting time of cementwhen it is mixed with water.Then, it is grounded to a fine powder andthen the cement is stored in storage bins orcement silos or bagged.Cement bags should be stored on pallets ina dry place.
44 THE CEMENT MANUFACTURING PROCESS quarrydumperloaderQuarry face1. BLASTING2. TRANSPORTcrushingstorage at the plantconveyor3. CRUSHING & TRANSPORTATION1. BLASTING : The raw materials that are used to manufacture cement (mainly limestone and clay) are blasted from the quarry.2. TRANSPORT : The raw materials are loaded into a dumper.3. CRUSHING AND TRANSPORTATION : The raw materials, after crushing, are transported to the plant by conveyor. The plant stores the materials before they are homogenized.
45 THE CEMENT MANUFACTURING PROCESS Raw grinding and burning storage at the plantRaw millconveyorRaw mix1. RAW GRINDINGpreheatingkilncoolingclinker2. BURNING1. RAW GRINDING : The raw materials are very finely ground in order to produce the raw mix.2. BURNING : The raw mix is preheated before it goes into the kiln, which is heated by a flame that can be as hot as 2000 °C. The raw mix burns at 1500 °C producing clinker which, when it leaves the kiln, is rapidly cooled with air fans. So, the raw mix is burnt to produce clinker : the basic material needed to make cement.
46 THE CEMENT MANUFACTURING PROCESS Grinding, storage, packing, dispatch Gypsum and the secondary additives are added to the clinker.clinker storageFinish grinding1. GRINDINGsilosdispatchbags2. STORAGE, PACKING, DISPATCH1.GRINDING : The clinker and the gypsum are very finely ground giving a “pure cement”. Other secondary additives and cementitious materials can also be added to make a blended cement.2. STORAGE, PACKING, DISPATCH :The cement is stored in silos before being dispatched either in bulk or in bags to its final destination.
50 Properties of cement and tests 1. Fineness95% of cement particles are smaller than 45 micrometer, with the average particle around 15 micrometer.Fineness of cement affects heat released and the rate of hydration.More is the fineness of cement more will be the rate of hydration.Thus the fineness accelerates strength development principally during the first seven days.
51 Continue on FinenessFineness tests indirectly measures the surface area of the cement particles per unit mass :Wagner turbidimeter test(ASTM C 115)Blaine air-permeability test(ASTM C 204)Sieving using No. 325 (45 μm) sieve (ASTM C 430)
52 Fineness Testing On left, Blaine test apparatus. On right, agner turbidmeter
54 2. SoundnessSoundness is the ability of a hardened paste to retain its volume after setting.A cement is said to be unsound (i.e. having lack of soundness) if it is subjected to delayed destructive expansion.Unsoundness of cement is due to presence of excessive amount of hard-burned free lime or magnesia
55 Cont. on SoundnessUnsoundness of a cement is determined by the following tests:Le-Chatelier accelerated test(BS 4550: Part 3)Autoclave-expansion test(ASTM C 151)
57 3. ConsistencyConsistency refers to the relative mobility of a freshly mixed cement paste or mortar or its ability to flow.Normal or Standard consistency of cement is determined using the Vicat’s Apparatus. It is defined as that percentage of water added to form the paste which allows a penetration of 10 1 mm of the Vicat plunger.
59 Consistency Test for mortar using the flow table
60 4. Setting TimeThis is the term used to describe the stiffening of the cement paste.Setting time is to determine if a cement sets according to the time limits specified in ASTM C 150.Setting time is determined using either the Vicat apparatus (ASTM C 191) or a Gillmore needle (ASTM C 266).“Initial setting time” is the time from the instant at which water is added to the cement until the paste ceases to be fluid and plastic which corresponds to the time at which the Vicat’s initial set needle penetrate to a point 5 mm from the bottom of a special mould.
61 Cont. on Setting TimeASTM C 150 prescribes a minimum initial setting time of 60 minutes for Portland cements.“Final setting time” the time required for the paste to acquire certain degree of hardness. This corresponds to the time at which the Viact’s final set needle makes an impression on the paste surface but the cutting edge fails to do so.ASTM C 150 prescribes a maximum final setting time of 10 hours for Portland cements.Gypsum in the cement regulates setting time. Setting time is also affected by cement fineness, w/c ratio, and admixtures.
64 5. Early Stiffening (False Set and Flash Set) Early stiffening is the early development of stiffening in the working plasticity of cement paste, mortar or concrete. This includes both false set and flash set.
65 False SetFalse set is evidenced by a significant loss of plasticity, i.e. stiffening, without the evolution of much heat shortly after mixing.Stiffening caused by rapid crystallization of interlocking needle-like secondary gypsum.False set cause no difficulty in placing and handling of concrete if the concrete is mixed for a longer time than usual or if it is remixed without additional water before it is transported or placed.
66 Flash Set (quick set)Evidence by a quick and early loss of workability and it is usually accompanied by evolution of considerable heat from the hydration of aluminates.The workability can not be regained without the addition of water.
67 6. Compressive StrengthCompressive strength of cement is the most important property.It is determined by ducting compression tests on standard 50 mm mortar cubes in accordance with ASTM C 109.In general, cement strength (based on mortar-cube tests) can not be used to predict concrete compressive strength with great degree of accuracy because of many variables in aggregate characteristics, concrete mixtures, construction procedures, and environmental conditions in the field.Rates of compressive strength development for concrete, made with various types of cement, are shown in Fig
69 Strength Development of Portland Cement mortar cubes
70 7. Heat of HydrationIt is the quantity of heat (in joules) per gram of un-hydrated cement evolved upon complete hydration at a given temperature.The heat of hydration can be determined by ASTM C 186 or by a conduction calorimeter.The temperature at which hydration occurs greatly affects the rate of heat development.Fineness of cement also affects the rate of heat development but not the total amount of heat librated.
71 Heat of Hydration determined by ASTM C 186 (left) or by a conduction calorimeter (right).
72 Cont. on Heat of Hydration The amount of heat generated depends upon the chemical composition of cement. Following are the heat of hydration generated on hydration of the four compounds of cement.Compound Heat of hydration Remarks C3S 502 j/g--C2S 260 j/gMinimumC3A 867 j/g MaximumC4AF 419 j/g--C3S and C3A are the compounds responsible for the high heat evolution.The approximate amount of heat generated using ASTM C 186, during the first 7 days (based on limited data) are as follows:
73 Heat of hydration (kj/kg) TypeNameHeat of hydration (kj/kg)INormal349IIModerate263IIIHigh early strength370IVLow heat of hydration233VSulfate resistant310
74 Cont. on Heat of Hydration Cements do not generate heat at constant rate as illustrated in Figure 2-45 for a typical type I Portland cement
75 Stage 1:heat of wetting or initial hydrolysis C3A and C3S Hydration. 7 min after mixing.Stage 2: dormant period related to initial set.Stage 3. accelerated reaction of the hydration products. That determine the rate of hardening and final set.Stage 4: decelerates formation of hydration products and determines the rate of early strength gain.Stage 5: is a slow, steady formation of hydration products.
76 8. Loss on Ignition (LOI)The test for loss on ignition is performed in accordance with ASTM C 114.A high weight loss on ignition of a cement sample (between 900 to 1000ºC) is an indication of pre-hydration and carbonation, which may be caused by:Improper and prolonged storageAdulteration during transport and transferLoss on ignition values range between 0 to 3%
78 9. Density and Specific Gravity (ASTM C 188) Density is the mass of a unit volume of the solids or particles, excluding air between particles. The particle density of Portland cement ranges from 3.10 to 3.25 Mg/m3, averaging 3.15 Mg/ m3.It is used in concrete mixture proportioning calculations.For mixture proportioning, it may be more useful to express the density as relative density (specific gravity). On an average the specific gravity of cement is 3.15.
79 Storage of CementCement is moisture-sensitive material; if kept dry it will retain its quality indefinitely.When exposed to moisture, cement will set more slowly and will have less strength compared to cement that kept dray.At the time of use cement should be free-flowing and free of lumps.